The term 'boron' refers to the oxide B2O3. 'Borate materials' thus contain B2O3, they source it to glass-building during melting in the kiln. Boron is actually the potter's friend (because of his electronic-controller-equipped kiln) while as the same time it can be a scourge in industry (because they are forced to fast fire), we will see how that is.
Your boron glaze might melt alot earlier than you think
The porcelain mug on the left is fired to cone 6 with G2926B clear glossy glaze. This recipe only contains 25% boron frit (0.33 molar of B2O3). Yet the mug on the right (the same clay and glaze) is only fired to cone 02 yet the glaze is already well melted! What does this mean? Industry avoids high boron glazes (they consider 0.33 high boron) because this early melting behavior means gases cannot clear before the glaze starts to melt (causing surface defects). For this reason, fast fire glazes melt much later. Yet many middle temperature reactive glazes in use by potters have double the amount of B2O3 that this glaze has!
In pursuit of a reactive cone 6 base that I can live with
These melt-flow and ball-melt tests compare 6 unconventionally fluxed glazes with a traditional cone 6 moderately boron fluxed (+soda/calcia/magnesia) base (far left Plainsman G2926B). The objective is to achieve higher melt fluidity for a more brilliant surface and for more reactive response with colorant and variegator additions (with awareness of downsides of this). Classified by most active fluxes they are: G3814 - Moderate zinc, no boron G2938 - High-soda+lithia+strontium G3808 - High boron+soda (Gerstley Borate based) G3808A - 3808 chemistry sourced from frits G3813 - Boron+zinc+lithia G3806B - Soda+zinc+strontium+boron (mixed oxide effect) This series of tests was done to choose a recipe, that while more fluid, will have a minimum of the problems associated with such (e.g. crazing, blistering, excessive running, susceptibility to leaching). As a final step the recipe will be adjusted as needed. We eventually chose G3806B and further modified it to reduce the thermal expansion.
Let me count the reasons this glossy white cone 6 glaze is pinholing
First, the layer is very thick. Second, the body was only bisque fired to cone 06 and it is a raw brown burning stoneware with lots of coarser particles that generate gases as they are heated. Third, the glaze contains zircopax, it stiffens the melt and makes it less able to heal disruptions in the surface. Fourth, the glaze is high in B2O3, so it starts melting early (around 1450F) and seals the surface so the gases must bubble up through. Fifth, the firing was soaked at the end rather than dropping the temperature a little first (e.g. 100F) and soaking there instead.
Can a decal firing melt a glaze? Yes!
Typical zero-boron high temperature glazes will not soften in a 1500F decal firing. But low temperature glazes will (especially those high in boron). Even middle temperature ones can soften. G3806C, for example, is reactive and fluid, it certainly will. Even G2926B, which has high Al2O3 and SiO2, has enough boron to soften and sometimes create tiny pits. In serious cases they can bubble like the mug on the right. Why? Steam. It was in use and had been absorbing water in the months since it was first glaze fired at cone 03. The one on the left was not used, but it did have some time to absorb water from the air, it is showing tiny pits in the surface. Even if moisture is not present, low fire bodies especially may still have some gases of decomposition to affect the glaze. One more thing: Fire the decals at the recommended temperature, often cone 022.
Slow cooling vs. fast cooling on a cone 6 transparent glaze
These are the inside uppers on two mugs made from the same clay with the same clear glaze. The one on the left was fired in a large electric kiln full of ware (thus it cooled relatively slowly). The one on the right was in a test kiln and was cooled rapidly. This glaze contains 40% Ferro Frit 3134 so there is plenty of boron and plenty of calica to grow the borosilicate crystals that cause the cloudiness in the glass. But in the faster cooling kiln they do not have time to grow.
Can a cone 6 functional glaze having only whiting and feldspar melt enough?
This flow test compares the base and base-plus-iron version of a popular CM recipe called "Tenmoku Cone 6" (20% whiting, 35% Custer feldspar, 15% Ball Clay and 30% silica, 10% iron oxide). Although iron is not a flux in oxidation, it appears to be doing exactly that here (that flow is just bubbling its way down the runway, the white one also fires to a glassy surface on ware). It looks melted in the tray on the right but notice how easily it is scratching on the tile (lower left). This demonstrates that looks can be deceiving. Cone 6 functional glazes always have some percentage of a power flux (like boron, lithia, zinc), otherwise they just do not melt into a hard glass. Maybe a glaze looks melted, but it has poor durability.
Out Bound Links
In Bound Links